Fundamentals of Polymer Engineering
Embed Size (px)
Transcript of Fundamentals of Polymer Engineering
Fundamentals_of_Polymer_Engineering/Fundamentals of Polymer Engineering/57261_01.pdfIntroduction to the World of Polymers
K-r Is m E of polymers This word stems from Greek: Poly = many, mers = particles. So this
term describes a molecule composed of many identical parts, called mers. The large molecule is therefore termed: macromolecule. What is left for us, is the practical definition of the term many. The minimum considers hun- dreds of mers. However, there are no sigdicant mechanical properties below about 30 mers, while the useful average reaches 200-2,000 mers. If one wants to speak about molecular weights (which is usually done in chemistry) a broad range between 5,000 up to 2 x IO6 may be representative, while in some cases it may reach 10.
The sheer existence of such a broad range of molecular weights indicates that we deal with long molecules that have no fixed or standard length (or weight). This presents a most comprehensive difference between macromole- cules and the smaller molecules that are characterized by a smgle and fixed molecular weight (e.g. water = 18). Prior to delving deep into the world of polymers, it is essential also to explain the common term plastics. The name itself actually, describes the stage of processing the polymer while it is plastic or soft-enabling smooth flow and shaping. On the other hand, plas- tics (or the scientific term, plastomers) refer to the major group of polymers that in combination with various additives leads to materials of construction.
In addition to plastomers, polymers are also used as elastomers (rubber-
[ 2 ] Introduction to the World of Polymers
like), textiles, coatings and adhesives. Many polymers may appear in various utility groups, determined by the final desired composition. Because plastics use is dominated by polymers, many people do not care about the difference between those two terms, which are similar but by no means identical.
While the synthetic polymers are, for good reasops, of major interest in this book one should acknowledge the historical role of natural polymers since the beginning of mankind: in food [protein, starch and others); in cloth- ing (wool, cotton, silk); and in various other uses (cellulose for writing and natural resins for ornaments). Later (in the 18th century) the resin exuded from rubber trees (Hevea Braziliensis) turned into a very useful product in transportation (wheels and tires), in industry (conveyor belts) and in general uses, including toys. Even today, many natural polymers are still in use,
TABLE 1-1 Historical Development of Production of Synthetic Polymers
Polymer Year Polymer Year
Celluloid Phenolics Alkyds Aniline-formaldeh yde Cellulose acetate Urea formaldehyde Polymethyl methacrylate Ethyl cellulose Polyvinyl chloride (PVC) Polyvinyl acetate Pol yvin y lbut yral Polystyrene Polyethylene [LD) Polyamides (Nylon 6-6) Melamines Polyvinylidene chloride Polyesters (unsaturated) Silicones Polytetrafluoro ethylene
ABS EPOXY Polyurethanes Polyethylene (HD) Polycarbonate
1870 1909 1926 1926 1927 1928 1931 1931 1936 1938 1938 1938 1939 1939 1939 1939 1942 1943 1943
1946 1947 1953 1954 1958
Polypropylene Polyacetal (DelrinTM) Chlorinated polyether
Phenoxy Ionomers Polyphenylene oxide (NorylTM) Parylenes Pol ybut ylene Poly (4-methyl pentene) TPX Polybenzimidazole Polysulfones Polyethylene sulfide Trogamid-T Polyaryl ether Polyphenylene sulfide Polybenzimidazo benzophenan-
Aromatic polyamides (KevlarTM) Polyamide-imide (PAI) Aromatic polyester Polyarylate (ArdelTM) Polyether-ether ketone (PEEK) Polyetherimide ( UltemTM) Thermotropic polyesters (LCP)
1959 1959 1959
1962 1964 1964 1965 1965 1965 1965 1965 1966 1966 1968 1968 1970
1972 1973 1974 1978 1982 1982 1984
Introduction to the World of Polymers
reaching highly developed processing methods. However, modem industry is m a d y based on raw material that is suitable for mass production. Hence the vitality of the synthetic polymers.
In intermediate stages (the 19th century) polymers made by the modifica- tion of natural resins have appeared, the most prominent ones being the cellulose derivatives. Celluloid (obtained by nitration of cellulose ) represents the first semi-synthetic polymer. It became useful after compounding with a plasticizer (mainly camphor) to reduce its brittleness. Many cellulose deriva- tives are still currently in use (as plastomers, textiles or coatings) but the major development in the 20th century is definitely attributed to many fami- lies of synthetic polymers-the era of polymers.
Table 1-1 presents by historical year, the beginning of commercial produc- tion of the most useful polymers. While many useful polymers appeared in the 1930s, the process of introducing new polymers continued during the 1950s, 1960s and so on. It apparently takes about 10 years for a newborn polymer to reach maturity. During this period it has to undergo infant devel- opment and compete with other polymers or nonpolymeric materials. The major issue has become the tremendous cost of commercialization of a new polymer, because the period of research and development (including market- ing) is long and costly. In spite of all this, novel polymers appear every year, as long as they demonstrate uniqueness. However, there appears an increas- ing trend towards polyblends (mixtures of existing polymers). There is a dis- tinction between homogeneous polymers (homopolymers), consisting of identical mers, and heterogeneous ones made of a random combination of two (or more) mers, namely, the copolymers. The latter may involve various compositions differing in the type, concentration and order of the distinct mers in the macromolecule.
In conclusion, a wide array of polymers is already in use, so that a system- atic presentation of their chemical structure, as well as the relationship be- tween structure and behavior at the final stage, is essential.
[ 3 ]
1. Describe 3 products made of plastics. What are the advantages over other materials? State other options.
2. Describe 3 natural polymers and the scope of applications. What syn- thetic polymers may replace them and what are their advantages?
3. Describe 5 thermoplastic polymers and 5 thermosetting polymers.
4 ] Introduction to the World of Polymers
What are the principal differences between the two groups? Give details on the structure of the mer in each case.
4. Can you convert thermoplastic polymers to thermosetting polymers? Thermosets to thermoplastics? Describe hybrids.
5. Find the output of polymer production in the recent two years in the US. Give details of production of the major polymer families and state the changes for each of them.
6 . Which polymers are products from the coal industry and which are produced by the petrochemical industry?
Table of Contents1. Introduction to the World of PolymersProblems
Fundamentals_of_Polymer_Engineering/Fundamentals of Polymer Engineering/57261_02.pdfThe Chemistry of Polymers
IN THIS CHAPTER we deal with a very basic concept-from where does everything start? We begin with the raw materials for the polymer industry, the so-called monomers, and explain how they are produced. The process for polymer synthesis - polymerization - should be well understood regarding both the mechanism as well as the industrial technology. We avoid going into too many details but still point out the basic principles.
Polymerization reactions involve careful control of purity of monomers, ratio of reactants, special additives, temperature and pressure, separation and recovery. Each family of polymers represents a wide range of variables. They appear in a large number of grades, differing in molecular weght, distribu- tion, degree of crystallinity, size of particles and types of special additives. The polymer leaves the reactor as a powder or as pellets (often, after passing through extrusion and granulation). Some stabilizers are directly added in the polymerization or granulation stage. The polymer is then stored in big silos for homogenation. This process is mostly carried out at special compounding units, which are responsible for exact mixing and composition.
2.2 THE PETROCHEMICAL INDUSTRY
The petrochemical industry, that branch of the chemical industry which is based on the exploitation of the crude-oil distillation products, has turned
[ 6 I The Chemistry of Polymers out to be the leading industry in chemistry, wherein most monomers and polymers are produced. It was preceded by the coal industry, developed mainly in Germany and Britain during the 19th century. By decomposition of coal at high temperature (an anaerobic process called cracking) products llke acetylene, methanol, or phenol are derived. These chemicals serve as the primary source for an extended array of polymers.
Acetylene is derived from carbide, the latter obtained by a reaction be- tween lime and coke (the major solid fraction obtained from coal pyrolysis). The basic chemical reactions are as follows:
CaO + 3C --* CaCz + CO (2-1) CaC, + 2Hz0 + Ca(OH)z + HC=CH
Just another step leads to the manufacture of one of the oldest mono- mers -vinylchloride - along with other vinyl derivatives (including acryloni- trile).
CHsCH + HCl + CHz=CHC1 (vinylchloride)
Ethylene, which serves as a source of many other monomers, can also be synthesized by the hydrogenation of acetylene.
CHzCH + Hz + CHz=CHz (2-4) Methanol is obtained in another process, by oxidizing coke with steam to
form a mixture of carbon monoxide and hydrogen, as follows:
C + HzO -, CO + Hz (2-5) Next steps will lead to the formation of methanol via a catalytic reaction:
CO + 2Hz + CH30H (2-6) Methanol may be further oxidized to formaldehyde:
CHjOH + %Oz --* HCOH (formaldehyde)
A whole family of polymers is derived from formaldehyde: polyacetal (polymethylene oxide), phenol-formaldehyde, urea-formaldehyde and mela- mine-formaldehyde. It is interesting to note that the other components (phe- nol, urea and melamine) are also products of coal pyrolysis.
2.2 The Petrochemical Industry
Like many other aromatics, phenol is produced from another fraction of the cracking of coal, coal-tar. These aromatics serve as the basis for a large list of other polymers, like nylons, epoxides and polycarbonates, in addition to polystyrene and other styrenic derivatives (ABS, SB rubber) and polyesters.
The petrochemical industry (based on crude oil and partly on natural gas) essentially replaced the coal industry as the major source of monomers. This industry was developed in Europe during the 1950s, but started in the United States as early as 1920.
The lowest homolog in the paraffin family, methane (CH,), (derived from crude oil but frequently found in natural gas), serves as the basis for the manufacture of methanol:
[ 7 ]
CH, + H20 -+ CO + 3Hz (2-8) CO + 2H2 -+ CHBOH (2-9)
Alternatively, methane can be converted to acetylene, and through it to all kinds of monomers.
Currently, by cracking the light fraction naphtha (with a boiling point between gasoline and kerosene), the unsaturated gases that serve the primary monomers -ethylene, propylene and butylene - as well as aromatics (includ- ing phenol) are obtained. From these, many monomers are derived. By the 1960s, 90% of all organic chemicals were derived from oil, and this trend continued growing. Only 3% to 5% of crude oil is used as chemicals, while the major portion is utilized as fuel. The world forecast for production of petrochemicals during 1996 was:
Ethylene 65 million tons Propylene 40 million tons Butadiene 7 million tons Benzene 38 million tons Xylenes 28 million tons
Let us describe the routes to some selected monomers, produced by the petro- chemical industry.
Monomers Derived from Ethylene
(VCM) CH,=CHCI (vinyl chloride)
[ 8 ] The Chemistry of Polymers
CH2=CH2 + 2HC1 + Y 2 0 2 + CH2Cl-CH2Cl -+ CH,=CHCl + HC1
VCM can also be manufactured by an alternative reaction:
Styrene can be synthesized by reacting ethylene with benzene (the latter present in the aromatic fraction of the oil cracking process- benzene, toluene and xylene).
2CH2=CH2 + 2C6H6 -+ CbHS-C2H5 + CH,=CH I (2-13) C6H5
Styrene serves as the monomer for the well-known polymer-polystyrene. It also serves as the source of many copolymers, that is polymers made from two monomers at varying compositions, such as S A N = styrene-acryloni- trile; SBR = styrene-butadiene rubber (the major synthetic rubber); SBS = styrene-butadiene-styrene (a modern family of thermoplastic rubbers which are not cross-linked); and the well-known terpolymer ABS which is based on 3 monomers - acrylonitrile-butadiene-styrene.
Vinyl acetate (a monomer frequently used in adhesives and coatings) may also be synthesized by reacting ethylene with acetic acid:
H2C=CH2 + CH3COOH + CH2=CH-O-C-CH3 8
Monomers Derived from Propylene
Acrylonitrile is obtained by reacting propylene with ammonia:
Another important monomer, methylmethacrylate (acrylic), is obtained by reacting propylene with carbon monoxide, oxygen and methanol:
2.2 The Petrochemical Industry 9 ]
CH3 I + H2O I (2-16) COOCH3
H2C=CH + CO + Y 2 0 2 + CH30H + H2C=C I CH3
( M U )
Propylene also serves as the source of the epoxy polymer, via epichlorohydrin:
H2C-CH-CH2CL \ / (2- 171 0
Incidentally, by a series of oxidation reactions on propylene, a very useful poly01 (glycerol) can be derived. The latter serves mainly in polyfunctional thermosets such as alkyds that undergo cross-linking.
H2C=CH + O2 + H2C=C-C=0 +
CH3 I L L (2-18) H2C=CH-CH20H + H202 --+ CHZOH
I I CHOH
Phenol and Other Aromatics
Phenol is mainly derived from benzene, but can also be obtained from propylene. It serves as the basis for several important monomers, in addition to its direct use as a reactive monomer via condensation with formaldehyde. This first man-made polymer, phenol-formaldehyde, appeared in 1901 and bears the trademark Bakelite@, after its inventor Bakeland. By reacting phenol with acetone, bis-phenol A is obtained. This serves as the basis for the manu- facture of epoxy and polycarbonate.
[ 10 ] The Chemistry of Polymers
0 I I CH3
2C&I50H + H3C-&-CH3 + HO-Cd-14-C-C6H4-OH + H20
Urea is obtained by the reaction between ammonia (NH,) and carbon dioxide (CO,):
2NH3 + C02 + H2N-C-NH2 + H2O a (urea)
As stated previously, condensation between urea and formaldehyde leads to the formation of the polymer urea-formaldehyde. A third member in this series is the melamine, which will also react with formaldehyde leading to the polymer melamine-formaldehyde. Melamine may also be derived by thermal decomposition of urea.
Both monomers for the production of Nylon 6-6 (one of the earliest poly- amides) may be synthesized from benzene: adipic acid and hexamethylene diamine.
Phthalic acids (iso, tera and ortho) are manufactured in the petrochemical industry from the three isomers of xylene. These acids and the corresponding anhydrides are the major basis for polyesters and alkyds.
Needless to say, there are many monomers and we illustrated some of the most useful.
In conclusion, the petrochemical industry currently supplies most mono- mers, while the coal-cracking industry remains an alternative option.
2.3 MONOMERS: BUILDING BLOCKS FOR POLYMER MANUFACTURE
What is a monomer? Any material that is able to be polymerized (that is, can form macromolecules) possesses a unique chemical structure, which is termed polyfunctionality. The simplest case - representing a functionality of two-appears as the covalent double bond, resulting from electron sharing. The paraffins (like methane and its homologs) are unable to polymerize - due
2.3 Monomers: Building Blocks for Polymer Manufacture
to lack of a double bond-hence they are not considered to be monomers. Ethylene, on the other hand, represents the simplest and most commonly used monomer, essentially due to the existence of an aliphatic double bond that starts the polymeric chain.
CHz=CHz + -CHz-CHZ-
monomer n CHz=CHz + (CHz-CHz), (polymer)
The various mechanisms of polymerization will be described later. If the monomer contains two double bonds (as in butadiene and other dienes) the final polymer can remain unsaturated, as each unit (mer) includes one double bond.
Ethylene represents a whole family of monomers, called vinyls
I I H X
in which the substituent X is hydrogen (H). However, X may also represent other elements or radicals such as chlorine or other halogens; CH3 group in propylene; phenyl (benzene ring) in styrene; an esteric group (acrylics); the CN group as in acrylonitrile; and many others. Sometimes two (or even more) of the hydrogen atoms are replaced. A list of monomers that have the potential to be polymerized through an addition reaction is shown in Table 2-1.
Another mode of bifunctionality exists in cyclic monomers, where open- ing of the ring is the starting stage of polymerization. The most common monomer in this group is ethylene oxide:
The ring in order to be activated should consist of a number of sides ddfering from six. In both cases (double bonds or ring opening), the monomers are directly added into macromolecules.
Functionality is even more apparent in monomers that polymerize through a condensation reaction. Let us consider a condensation reaction of monofunctional groups, like classical esterification:
CH3COOH + HOC2H5 + H3CCOOC2HS + HzO (2-26)
[ 12 I The Chemistry of Polymers TABLE 2-1 Monomers Polvmerized by Addition
Code and Name Monomer
POM: Polyoxymethylene (Polyacetal)
PB: Polybutene- 1 (Polybutylene)
HC=CH2 I CH3
CH, I C=CH2
CH3 I C=CH2 I COOCH,
HC=CH2 I OH
CH, CH3 I
CH=CH2 I CH,
C1, C =CH,
CH=CH2 I OCOCH3
CH=CH2 I cfi H,
2.3 Monomers: Building Blocks for Polymer Manufacture
It is apparent that two reactants-@ organic acid and an alcohol) consisting of single reactive (functional) groups of opposing nature (OH = hydroxyl and COOH = carboxyl) -neutralize each other. The resultant product is an es- ter, and one molecule of water is eliminated. This reaction also resembles the neutralization of an acid by a base (forming a salt) in inorganic chemistry; however, there is no sequence or chain reaction, so there is no polymer. If we want to build a polymer chain, at least bifunctional reactants are essential. In the case of the ester, a dicarboxylic acid and glycol are reacted-again via condensat ion.
[ 13 ]
HOOC(CH2)4COOH + HOCHz-CHzOH + HOOC (CH2)4COOCHzCH20H
The uniqueness of this ester is the retention of two opposing groups at the ends, which actually enables more and more reactions, thus building a large ester molecule - a polyester.
n[HOOC(CH2)4COOH] + n(HOH,C -CH,OH] -+ (2-28) HO[OC(CH,)4COOCH,CHzO]nH + (2n - 1) HzO
In conclusion, the existence of at least two functional groups is a neces- sary (yet not sufficient) requirement for a small molecule to act as a mono- mer. The repeating unit - the mer- is not necessarily identical to the mono- mer. Such an identity exists only in addition polymerization, wherein the monomer molecules llnk up without any elimination. In the case of polyes- terification (as well as with other similar condensation reactions) elimination of small molecules is involved (in most cases water). That is the source of the name - condensation polymerization- a small molecule is evolved or con- densed. The term stepwise polymerization is more commonly used. This will be explained later.
Another example of polymerization by condensation is the formation of polyamide (in our case Nylon 6-6) by reacting a di-acid with a diamine.
n[H2 N (CH,), NH, + n[HOOC (CH,), COOH] -+ (2-29) H [HN (CHZJ~NHCO (CH2)4CO]nOH + (2n - 1) HzO
It is also possible to polymerize by condensation a single monomer with two opposing groups at its ends. In the case of a polyamide, Nylon 6 can be polymerized from the monomer H,N(CH2)5COOH
n[H2N (CH,), COOH] -, H[HN (CH,), CO],OH + (n - 1) HzO (2-30) In practice, the cyclic caprolactam anhydride serves as the common mo- nomer.
[ 14 I The Chemistry of Polymers
The rate of polymerization is dependent on the structure of the monomer and the substituent groups, the right use of catalysts and initiators, and the appropriate conditions. All this will be thoroughly discussed in the next section that deals with the mechanism of polymerization.
Table 2-2 describes some monomers that polymerize by stepwise reac- tions (mostly condensation).
2.4 POLYMERIZATION-THE MECHANISM OF THE PROCESS
There are many mechanisms describing the process of polymerization (two of which were already discussed- addition and condensation). These terms describe only the chemical process, not the major engineering aspect - the rate of the reaction (kinetics). Therefore, it is beneficial to differentiate between two major polymerization routes- chain polymerization and step- wise polymerization.
Chain polymerization is mainly represented by the addition reaction and is characterized as follows:
1. Long chains appear at the early stage. 2. Monomers are added to long chains, and steadily disappear during the
3. There is no elimination of small molecules. 4. Quite high molecular weights may be obtained ( lo5 to 2 x lo6). 5. Extension of polymerization only increases conversion not the chain
On the other hand, the kinetics of stepwise polymerization differ com- pletely, accordmg to the following:
1. At the early stages dimers, trimers, and tetramers are formed, by react- ing pairs of opposing functional groups, so that the growth develops in stages.
2. Monomers disappear in the early stage. 3. There is (usually) an elimination of a small molecule. 4. Molecular weights are low to medium (below 50,000 normally) . 5. Extension of the polymerization increases both conversion and molec-
2.4 Polymerization-The Mechanism of the Process [ 15 ]
TABLE 2-2 Monomers Reacting by Stepwise Polymerization Polymer Monomers
PES: Polyester (PET: Polyethyleneterephthalate) Typical group
PA: Polyamide (Nylon 6-6) Typical group
(Note: here there is no condensation.) PC: Polycarbonate Bis-phenol A
HOCH, - CHZOH HOOCC, H,COOH -co-0 H,N(CH2)6NH2 HOOC (CH,),COOH -NH-co-
HO ( CH,) ,OH OCN(CH,),NCO -NH-co-0-
CH, I I CH3 0
HO- C a 4 - C - C, H, - OH
Phosgene C1- k -C1 ChHSOH HCHO
N / \\
I L L \ N
N H Z
Stepwise polymerization includes most condensation processes, but also some reactions involving ring opening, and even addition reactions (typified by the formation of polyurethane from a di-isocyanate and a di-alcohol). The viscosity serves as a sensitive indication of the growth of the polymer. There- fore, in stepwise polymerization the viscosity of the system increases slowly and reaches high levels only toward the end of the reaction. In chain polymer-
[ 16 ] The Chemistry of Polymers
ization, high viscosity material appears at the initial stages, indicating a mixture (or solution) of long chains with yet unpolymerized monomers.
Chain (Addition) Polymerization
With this background, let us explain the mechanism of chain (addition) polymerization. If we write the electronic structure of the main group, vinyl:
H H H H H H
c=c 4 c : : c . . . . . . . .
4 -c : c . I I c . . . .
H X (A)
k k t H X t 1 H H
- : c : c + . . . .
In configuration (A) one pair of electrons in each monomer unit is unpaired (in the ?r-orbital), which enables a smgle electron to react with an external single electron and end up as a free radical. This is the key to the most conventional mode of polymerization, via free radicals. Configuration (B) leads to an excess of electrons on one side (anion) and a shortage on the other side (cation). This leads to ionic polymerization (cationic or anionic). Hence there are choices of various mechanisms for polymerization, where the chem- ical nature of the monomer (characteristics of the substituent groups) dictates the preferred mechanism. This is shown in Table 2-3.
TABLE 2-3 Initiation in Chain Polymerization
TYPE OF INITIATION
Radical Cationic Ionic Stereospecific
Ethylene Styrene 1-3 Dienes Halogenic olefins, TFET Vinyl esters (VAC) Isobutylene; vinyl ether Aldehydes, ketones Butene-1, propylene Acrylics, acrylonitrile
+ + + + + + + + +
- + + -
- - - -
+ + + + + + -
+ + -
+ 'will be discussed later
2.4 Polymerization-The Mechanism of the Process
We begin with radical initiation because it is most commonly used. In order to activate the monomers, materials that release free radicals are called on, known as the free radical initiators. (It should be stressed at the outset that the term initiator differs from the term catalyst, because the former becomes part of the generated molecule, as will be described later. A catalyst does not participate directly in the chemical reaction, but speeds it up.) In order to understand the mechanism of polymerization via free radical initia- tion, we write the relevant chemical equations.
kd I + 2R*
ki R * + M + R M *
where I = Initiator (concentration)
R* = Free radical (concentration) M = Monomer (concentration)
RM* = growing chain radical
A common initiator is benzoyl peroxide BPO (C6HsCOO)2, which decom- poses at 80-95OC to form free radicals, as follows:
Another useful initiator is azobiisobutyronitrile (AZBN) which decom- poses at 50-70C, as follows:
The reaction between the free radical and the monomers completes the stage of initiation:
(CH3)2C* + H2C=CHX + (CH3),-C--CH2-(!2* CN I k I CN
[ 18 ] The Chemistry of Polymers
It is apparent that a fraction of the initiator is retained in the chain radical, which will eventually continue to grow according to the steps of propagation and termination.
k, RM' + M -+ RMM'
k, RMM* + (n - l)M -+ R(M),M*
This equation represents a whole series of reactions, wherein the mono- mer reaches (by diffusion) the chain radical and is attached to the growing chain. All this may happen during fractions of a second and lead to a giant chain, with a free radical at the end. A process is now needed that will terminate the large chain- the termination reaction.
k,, RM,M' + RMmM* -+ RM,+,+zR
kt,d RM,M* + RMmM' -+ RM,+lH + RM,CH=CHX
Combination, shown in equation 2-39, occurs more frequently and leads to longer chains. In essence, during combination two growing chain radicals meet and combine to form a smgle chain. When the process is disproportiona- tion, the reaction between two growing radicals yields two polymeric chains (one unsaturated).
It is obvious that all three reactions (initiation, propagation and termina- tion) are vital for the polymerization process, but the propagation step deter- mines both the rate of the polymerization process and the chain length (as defined later). The rate of propagation (actually representing the rate of po- lymerization), r,, depends on the rate constant k, and on the concentration of reactants. It is, in principle, identical to the rate of disappearance of the monomer.
rp = -dM/dt = k,(M)(M*) (2-4 1)
This is virtually true, since for each chain radical of size n (mers), only one monomer reacts at the initiation step, and (n - 1) monomers react during the propagation steps.
2.4 Polymerization-The Mechanism of the Process
It is normally assumed (and verified experimentally) that the free radicals reach a constant concentration (steady-state assumption) so that the rate of initiation, ri, equals the rate of termination, r,:
[ 19 ]
r1 = 2 f I (rate of initiation) (2-42)
where f expresses the efficiency with which free radicals formed by Equation (2-33a) react by Equation (2-33b).
r, = 2 k, (M*)2 (rate of termination) (2-43)
Taking ri = r, , M* can be expressed as: 0.5
M = &] (2-44) This leads to a final expression for the rate of polymerization (identical to rate of propagation).
The rate of polymerization is proportional to the concentration of the mono- mer and to the square root of the concentration of the initiator.
The kinetic constants are mainly sensitive to the temperature, mostly through the Arrhenius relationship:
k = bexp (-EIRT) (2-46)
where E = energy of activation, R = gasconstant T = temperature in Kelvin.
Equation (2-46) defines a straight-line with a negative slope, on a semi- logarithmic scale, (1n)k versus UT. The slope ( -E/R) indicates the sensitivity to the effects of temperature. The combination of the constants in Equation (2-45) leads to a large positive value for E, which means a very hlgh sensitivity to an increase of temperature. The rate thus increases roughly two fold to three fold with a 10C enhancement in temperature.
How is the chain length estimated? If we define the instantaneous chain length as the ratio between the rate of propagation and rate of termination, we reach an expression for the kinetic degree of polymerization, DP, (equiva- lent to the number of mers in the chain) as follows:
[ 20 I The Chemistry of Polymers
Equation (2-47) holds for the case of termination by disproportionation, while when combination prevails the value should be doubled. The instantaneous molecular weight (MW) of the polymer chain is derived by multiplying DP by the molecular welght of the repeat unit.
The major difference between the expressions for rate of reaction and the degree of polymerization is that the latter depends on the inverse of the square root of initiator concentration. The reason for that is obvious, as more initiations of chains lead to shorter ones. On the other hand both rate and MW are proportional to monomer concentration. Therefore, in a batchwise process the highest rates and molecular weights occur at the outset, while later the concentration of the monomer will gradually diminish. The concen- tration of the initiator varies little throughout the polymerization process.
The combined constant K differs from that for the rate function (K), resulting in a negative activation energy, so that an increase in temperature will decrease MW. This fact should be considered when controlling the tem- perature in the reactor, as most reactions are exothermic, and efficient ways for the absorption of the heat of reaction are essential. There are alternatives for free radical formation that come from other sources of energy such as light, heat, or high-energy radiation.
In addition to the three principal reactions that prevail in radical polymer- ization, a fourth one often occurs, that is, the chain transfer reaction. In this case the free radical passes from the growing chain to another molecule (usually a small one llke an active solvent, the monomer itself, or even to a polymeric dead chain) leading to the termination of one chain together with the starting of a new one that is capable of growing.
RM,M* + XA + RM,+IX + A* (2-48) XA = a small molecule (solvent or even contaminant)
A* + M + AM* (newgrowth) (2-49) RM,M* + M -, RM,+l + M* (transfertomonomer) (2-50) An interesting result is observed. On one hand, a chain is terminated and
thus shortened, while on the other, the total rate of the process may be barely affected. However, if the new radical A* is not able to polymerize, it can only react with another radical into a simple molecule. This process called inhibition, often serves as a means of eliminating premature polymerization of the monomer during storage and transportation.
2.4 Polymerization-The Mechanism of the Process [ 21 ]
A* + A* -+ A-A (2-51)
When chain transfer occurs to a finished polymer, branches are formed. This phenomenon is found in low-density polyethylene, which exhibits vari- ous kinds of branches extending from the main chain.
RM,M* + P -+ ~UVI,+~H + P' (2-52) where P = polymer chain
P* + M -+ CH2-CH2-CH-CH2 (polyethylene with branched radicals)
In conclusion, the transfer reaction leads either to the shortening of the chain or to the formation of side branches. In both cases many physical properties will be affected, as shown later. However, it is possible to harness this reaction under controlled conditions as a chain-transfer regulator, a re- tarder or inhibitor. The theory of polymerization kinetics has reached a high level of development, which enables an improved engineering design of the process and good control on the rate, molecular weights and their distribu- tion, and the existence of secondary reactions.
Ionic Polymerization Differing slightly from the free radical mechanism that has been widely discussed, ionic polymerization uses specific catalysts to serve as electron withdrawing agents (Lewis acids and others), forming a positive ion (cation) properly named carbonium.
Whenever the catalyst serves as an electron donor (like amines), a negative ion (anion) is formed-carbanion.
N H 2 + M + NHzM- (2-56) The propagation stage resembles in principle that of free radical propaga-
tion, but termination is totally different because the two chain ions bearing
The Chemistry of Polymers
the same sign cause repulsion, as opposed to the attraction that is essential for termination. Therefore the mechanism of termination is much more com- plicated, and the growing ion has to react with a counterion or in a transfer reaction. In some cases, there are no conditions for transfer, so that the final ionic chains are still reactive (so-called living polymers). They may continue to grow eventually if a new monomer is provided. In practice this unique phenomenon is exploited in anionic polymerization without termination for well-defined and ordered homopolymers or copolymers.
In principle, the appearance of electron donor groups near the double bond of the monomer leads to a cationic mechanism, while positive groups that withdraw electrons mostly lead to the anionic process. An increase of temper- ature usually leads to a decrease in rate of reaction or length of the chain. Polymerization always occurs in solution, wherein the solvent acts as separa- tor of the ion-pair, and quite often as a transfer reagent. As already mentioned, most monomers undergo polymerization via free radicals, mainly when con- jugated double bonds are present or substitute groups that withdraw elec- trons.
The coordinative (stereospecific) polymerization mechanism differs from the previous ones. It caused a real revolution in the polymer world when developed in the 1950s by the scientists Ziegler (in Germany) and Natta (in Italy)-both Nobel Prize Laureates in 1963. The principle here is the use of specific catalysts that orient the mers in the chain into a highly ordered configuration. By this mechanism, ethylene forms a linear (branchless) chain, so-called high density polyethylene (specific mass 0.95 to 0.96) which was developed by Ziegler.
Propylene (and other vinyl monomers) form highly ordered structures, termed isotactic, wherein all the side groups (methyl) appear on the same side of the plane.
CH3 CH3 CH3 I
-CH -CH2-&H-CH2-&H-CH2- (isotactic polypropylene) (2-57)
Another ordered configuration is termed syndiotactic, which is an alternat- ing structure.
Both structures exhibit a high degree of crystallinity in contrast to disor- dered polypropylene (atactic) wherein the methyl group appears randomly in either side of the plane of the chain backbone.
2.4 Polymerization-The Mechanism of the Process 23 ]
CH3 CH3 I
- CH - CH2- LH- CH2- CH- CH2 -CH- CH2- (2-59) I CH3
This latter polymer is commercially useless.
family, is the polybutylene (polybutene- 1). Another ordered polymer, which appears as a new homolog in polyolefin
CH3 I CH2 I
[ - CH-CH21, (polybutane- 1)
Many polymers may be formed by this novel method into highly ordered and highly crystalline chains. The catalysts developed by Ziegler and Natta are composed of a combination of organo-metallic compounds (metals from Group I-III in the Periodic Table) and halogen derivatives of transition metals (Groups IV-VIII), such as the combination (C2H5)3Al with TiC13. They form a complex structure that binds the monomers into a preordered position. In spite of the tremendous achievements in this field, the exact mechanism is in dispute, since the theory is complicated.
As stated in Section 2.4, the condensation reaction may be the basis for the mechanism of stepwise polymerization. As long as the functionality equals 2 (di-acid and di-alcohol in polyester or di-amine in polyamide), only linear chains are obtained. However, once polyfunctionality prevails (appear- ance of tri-alcohol like glycerol, or tri-acid), reactive branches are formed that may interact and lead to a three-dimensional structure, called cross-linked (gelation). This is the basis for thermosetting polymers on one hand, or for stabilizing the elastomeric chain on the other hand (replacing vulcanization).
Lets designate the number of functional groups of the same type by N. If No functional groups existed at the beginning of the polymerization process and, during the reaction, molecules from group A are being depleted by the counter group B, so that a single group of either type is retained at the ends of the growing chain, then:
[ 24 ] The Chemistry of Polymers
The degree of conversion (P) is expressed by
P = (No - N)/N, (2-6 1)
On the other hand, the extent of the chain (the number of repeating units = mers) is expressed as DP = average degree of polymerization.
(2-62) - DP = N,/N
The explanation is that we started with No groups and ended up with N groups, all at the ends of the chains. The relationship between degree of polymerization and conversion, is derived:
- DP = 1/(1 - P) (2-63)
The conclusion is that a very high degree of conversion is needed in order to gain significant molecular weights.
MW = DP x M, (2-64)
where M, = mass of repeat unit. Once two monomers (with opposing functionality) interact, the average
value for M, equals half of the mass of the repeat unit. Equation (2-63) points out how difficult it will be to reach high molecular weight materials via condensation reactions. Looking, for example, at the formation of polyamide Nylon 6-6.
NH&H2)6 NHH + n HOOC(CH2)4COOH + (2-65) H[HN(CH,)&HCO(C H2)4CO], OH
For P = 0.99, DP = 100 (from Equation 2-63).
M, = 1/2 HN(CH2)6HNCO(CH2)4C0 = 113, therefore, MW = 11,300.
In reality, the highest obtainable MW is around 50,000. In addition to the requirement of a very high conversion (which also calls for a long time) it is crucial to avoid a surplus of any of the reactants or the presence of mono- functional groups and contaminants. All of these may nul& a functional group and just substitute it-thus making this end of the growing chain inactive. This requires strict efforts for equivalent functionality (stochiome- tric ratios). Any side product (mostly water) must be removed, otherwise a reverse reaction may operate (depolymerization).
2.4 Polymerization-The Mechanism of the Process [ 25 ]
We have been discussing the mechanism of polymerization of a single monomer (homopolymer). However, when two or more monomers polymer- ize in situ, the chains obtained differ in composition and location of each mer. These are controlled by the ratios between the tendency to homopoly- merize and to cross-polymerize rl and r,. (Details will follow.)
A random chain constructed by monomers A and B via an addition reac- tion looks as follows:
(It is important to stress that the polymers obtained via condensation are not copolymers, as their repeat unit is identical.)
The importance of the reactivity parameters rl and r, is revealed if the four basic reactions for a copolymer chain (by free radicals, as an example) are expressed as follows:
kll , AA* kl2 > AB*
(1) A* + A (2) A* + B (2-66)
Reactions (1) and (3) are identical to homopolymerization. The parameters rl and r2 are defined as the ratio between the kinetic constant for homopolymer- ization and that for cross-reaction.
rl = kll/k12 r2 = kz2/kzl
The rate of disappearance of monomer A (-dA/dt) will be derived from Equation (2-66) (1) and (4), while that of B (-dB/dt) is derived from reactions (2) and (3). By dividing both rates, the ratio dA/dB is obtained, and that de- scribes the instantaneous composition ratio of the two mers in the chain. Lets call this ratio dAldB = Y, whereas the appropriate ratio of molar concen- tration in the mixture of the monomers will be termed, X = AIB. The expres- sion for the composition in the chain Y (ratio) as related to the ratio of the monomer feed (X) represents the so-called equilibrium equation.
The composition of the feed varies in a batch reaction, but keeps constarit in a continuous one. In any case, the instantaneous composition of the copol- ymer (Y) and monomer feed (X) is expressed as:
[ 26 ] The Chemistry of Polymers
X(r,X + 1) r2 + X Y = (2-67)
Equation (2-67) has a deficiency in graphical presentation, as the ratios Y and X are bounded between zero and infinity. Therefore, it is better to normal- ize by using mole fractions in the polymer:
dAI(dA + dB) = F1 = YI(1 + Y) and in the monomer mixture
f l = A/(A + B) = XI(1 + X) In a binary system (copolymer)
f , + f, = 1 F1 + F2 = 1
The boundaries for mole fractions are 0 and 1. Equation 2-67 is transformed to:
While both Equations 2-67 and 2-68 are very useful, the graphical presenta- tion of Equation 2-68 is advantageous, (as shown in Figure 2-1).
0 f l 1
FIGURE 2-1 Equilibrium curve for copolymerization
2.4 Polymerization-The Mechanism of the Process
The diagonal (F, = f , ) serves as the reference line. This line represents the unique case where r, = r2 = 1, which leads to Y = X in Equation 2-67, or F, = f , in Equation 2-68. In this unrealistic case, the composition of the copoly- mer is identical to that of the monomer mixture.
Another extreme case is described wherein rl = r2 = 0, which means that none of the monomers is polymerizable by itself, and yet a copolymer is ob- tained. Equations (2-67) and (2-68) verdy in this case that Y = 1 and F1 = 0.5 (always 50% of each component). This structure, named alternating, may be identified upon examining the chain:
[ 27 ]
as there is no way to produce AA or BB bonds. The most common structure is the random chain
where the exact composition will be dictated by r, and r,. The intersection between the equilibrium curve and the diagonal is called
the azeotropic point (resembling that in binary distillation) in which Y = X or F1 = f , . The conditions for an azeotrope may be found by using Equation (2-67).
1 - r2 y = x = - 1 - rl (2-69)
which requires that both r, and r2 are either smaller or larger than 1 (see curves 2 and 3 in Figure 2.1). Curve 1 applies when r, > 1 and no azeotrope exists. In this case, the copolymer is always richer in A as compared to the composition of the monomer feed mixture. If r, and r2 are quite large, one obtains block copolymers,
Another configuration is called a graft copolymer, wherein one monomer appears as a branch on the main chain, consisting of the other
I B B B B B B
Needless to say, by copolymerization a wide variety of structures and com- positions may be derived. Copolymers are widely used in elastomers and
[ 28 ] The Chemistry of Polymers
artificial textiles, as in many plastomers. The most common are S A N (sty- rene-acrylonitrile); SB (styrene-butadiene); EP (ethylene-propylene); Saran@ (vinylchloride-vinylidene chloride); or ABS (a terpolymer comprised of acrylo- nitrile, butadiene and styrene).
2.5 POLY MERIZATION-I N DUST RIAL PROCESSES
Transfer of the polymerization process from the laboratory to a full scale industrial level calls for the solution of many engineering problems- the structure of the reactor, removal of heat and thermal control, mixing of a high viscous mass, etc. In spite of the advantages of a continuous production line, there are still batch reactors in use, mainly for small scale production. In the condensation polymerization process, some aspects must be carefully followed - exact stochiometric balance between reactants (and prevention of loss of either monomer); elimination of by-products (water or other small molecules) sometimes by employing vacuum; prevention of decomposition by oxidation at high temperatures (use of an inert atmosphere); and control- ling premature gelation.
These processes are frequently batchwise, while viscosity increases gradu- ally up to the final stages. In most cases separation between monomers and polymer is unnecessary. On the other hand, polymerization processes based on free radical initiation involve strongly exothermic reactions that call for critical control of temperature and removing heat from highly viscous sys- tems. In most cases, separation of excess monomer is essential as well as polymer separation from the dispersing fluid.
If possible from the point of view of efficiency, polymerization of the reactants without any use of a dispersing medium is desired. This method is called Bulk Polymerization. However, in order to absorb the heat released in the reaction, other methods like suspension or emulsion polymerization are frequently used. In this case, the water absorbs heat and provides good control of temperature. Another (less popular) method is the solution (homogeneous or heterogeneous) polymerization, which is mostly utilized in ionic initia- tion. We compare advantages and disadvantages of each method. (Table 2-4 describes the most useful polymerization methods for some commercial poly- mers).
This method is simple to operate, efficient in regard to reactor space utilization, and leads to a polymer that is pure without the retention of other species. On the other hand, the absorption of heat is quite difficult, leading to the danger of overheating that prevents controlled production. There is
2.5 Polymerization- Industrial Processes [ 29 I TABLE 2-4 Methods of Industrial Polymerization
Polymer Bulk Solution Suspension Emulsion
PVC + + + + + + PS + + + + + PE + + + + + PP + +
ABS + + Acrylics + + + + +
Nylon + +
also a high energy demand for mixing a stirred reactor, as a result of the very high viscosity. In a tubular reactor, comprised of many small diameter tubes, the absorption of heat is easier, but polymerization temperature is less con- stant, causing a wider molecular weight distribution. Overheating may also lead to the phenomenon of self-acceleration. This method is mainly used in condensation processes, but is also adopted in the production of polyethylene and PVC, as well as in monomer casting operations in molds with acrylics.
This method enables good control of temperature while the viscosity of the system drops. It is also sometimes advantageous to utilize the polymer product in solution, as with coatings and paints. On the other hand, both chain length and rate of production decrease, as a result of the diminished concentration of the monomer. Other problems are related to solvent reten- tion and recovery, and hazards of fire and health.
This is a popular method (mainly in PVC) that improves control, while circumventing some of the disadvantages of the former methods. The product is obtained as pearls that are handy for further processes. In suspension polymerization some additives (stabilizers) are needed, enabling the disper- sion of monomer droplets and preventing coagulation. When stirring stops, the polymer precipitates. The reaction occurs in the monomer droplets in which the initiator is dissolved. Efficient drying and elimination of dispersing additives are crucial.
[ 30 I The Chemistry of Polymers Emulsion Polymerization
This is an important method that, in addition to improved thermal con- trol, results in a higher rate of production, higher molecular weights and a narrow distribution. The product may be utilized as an emulsion like rubber latex or coatings. Otherwise the emulsion must be destroyed, and the poly- mer carefully dried and separated, because retention of residues from the emulsifier (detergent) may cause the deterioration of properties (mainly for electrical uses).
The kinetics of emulsion polymerization differ completely from that of bulk or suspension. The soap (detergent) is used not only as a stabilizer but mainly as locus of the polymerization- so-called soap micelles. These consist of an array of 20-100 molecules of soap creating a micellar structure of 25-50 A in length (radius). The initiator is water soluble and the free radicals and the monomer molecules diffuse into the hydrophobic interior of the micelles while water is attracted to the hydrophilic exterior zone. Thus, the micelles serve as the core of growing polymer particles. At a later stage the micellar structure disappears, and the process continues in the polymer particles swol- len by monomers, leaving the soap as a protective layer on the particle sur- face. The concentration of soap dictates the molecular weight and rate of production.
1. Define the term chain length. If two polymers have the same chain length, do they also have the same molecular weight?
2. What is the molecular weight of PVC which has 750 mers?
3. Is polyester a copolymer?
4. In the case of a polymer made by condensation, is the repeating unit identical to the sum of the monomers?
5. What is the molecular weight of a cross-linked polymer. How are cross-linked polymers dissolved?
6 . In a polymerization process where there is no change in the viscosity
Problems [ 31 ]
during initial 2 hours and then a rapid rise occurs, what is the mechanism? What is happening in the first two hours?
7. In a polymerization process where the viscosity rises slowly for sev- eral hours and then stabilizes, what is the mechanism? What is the sigmfi- cance of measuring the viscosity?
8. A petrochemical plant manufactures polyethylene by free radical ini-
a. Increase the rate of polymerization by 50%, without changing the monomer concentration. How does it affect the molecular weight?
b. Increase rate of polymerization by 100% and molecular weight by 20%. Hint: change concentrations of both monomer and initiator.
c. Decrease molecular weight without changing concentrations. Of- fer two options with no calculation.
tiation in a continuous process. Solve the following changes:
9. What is the significance of termination in addition polymerization? What happens when a transfer reaction replaces the termination? What hap- pens when neither termination nor transfer occur?
10. A polymer is manufactured from the monomer HO(CH&,COOH. a. What is the generic name of the polymer? b. What is the mechanism of polymerization? c. What is the molecular weight when conversion is 95%, 989'0, 99%? d. Is it possible to reach 100% of conversion?
11. A copolymer is made from vinyl chloride and vinyl acetate, so that the molar concentration of the acetate in the polymer is 5%. What is the composition of the feed? Plot an equilibrium curve.
r1 = 1.4 Data: vinyl chloride (1) vinyl acetate (2)
r2 = 0.65
12. Plot an equilibrium curve and modlfy the basic equation for the fol- lowing cases of copolymerizations:
a. rl = r2 = 1 b. rl = r2 = 0 c. rl = r2
[ 32 ] The Chemistry of Polymers
13. Compare the following polymerization processes and define the differ- ence in the product properties. The polymer is PVC via free radical initiation.
a. Bulk polymerization. b. Suspension polymerization. c. Emulsion polymerization. d. Solution polymerization.
Table of Contents2. The Chemistry of Polymers2.1 Introduction2.2 The Petrochemical IndustryMonomers Derived from EthyleneMonomers Derived from PropylenePhenol and Other Aromatics
2.3 Monomers: Building Blocks for Polymer Manufacture2.4 Polymerization - The Mechanism of the ProcessChain (Addition) PolymerizationInitiationPropagationTerminationTransfer ReactionsIonic Polymerization
2.5 Polymerization - Industrial ProcessesBulk PolymerizationSolution PolymerizationSuspension PolymerizationEmulsion Polymerization
Fundamentals_of_Polymer_Engineering/Fundamentals of Polymer Engineering/57261_03.pdf3 C H A P T E R Structure and Ch ara c t eriza tion of Polymers
3.1 THE CHEMICAL STRUCTURE
THE CHEMICAL STRUCTURE of the homopolymers consists of an exact repetition of the chemical structure of the mer unit. The chemical bonds are mostly primary covalent ones, mainly C-C and C-H , but include also C-0, C-N, and so forth. There appear also various isomers, double bonds (unsaturation), tertiary or quaternary carbons, ring-llke structures, and others. There are also secondary bonds, albeit weaker than the primary ones. One typical isomer, found in polymers, is based on the presence of head-to- tail bonds as compared to head-to-head or tail-to-tail bonds. This is illus- trated by the vinyl group, with the substitute radical -X.
CHz-CH- CH2-CH-CHZ-- CH- (head-to-tail structure) I X
I X I X or
-CHz-CH-CH-CHz-CHz-CH-CH-CHz- I 1 x x
(tail-to-tail and head-to-head structure)
I 1 x x
[ 34 ] Structure and Characterization of Polymers
The head-to-tail isomer occurs more frequently. Other types of isomers may be defined under the heading of chain architecture. The nature of the substituent group dictates the polymer behavior, m a d y through secondary intermolecular bonds or rotation around this bond. That determines the flexi- bility of the chain, its mechanical strength, and the chemical affinity (com- patibility) to other compounds (solvents, plasticizers and other additives). Taking for example the substituent group of the halogens (X = F, C1, Br, I), it is well known that the strength of the primary bond diminishes from fluorine to iodine, respectively. Hence, the fluorocarbon polymers present excellent thermal and chemical stability (including weather resistance). Polyvinylchlo- ride is affected mainly by its polar secondary bond and is, therefore, more rigid than polyethylene, while the polymers based on bromine or iodine are unstable. The bromine derivatives, however, are most efficient as fire retard- ants because of their weaker bonds. Strong secondary bonds result from the existence of polarity (dipole-moment, as in the case of PVC) or from hydrogen bridges (as in the case of polyamides).
Nylon 6-6 I
(hydrogen bridge) H t 0 0
The basic chemical structure, including end groups, obviously determines the chemical behavior, that is, resistance to various chemicals such as acids, bases, salts, and organic solvents. As an example, polyamides (Nylon) are sensitive to acidic hydrolysis because of their chemical structure. On the other hand, the existence of hydrogen bridges produces a compact, highly crystalline structure, with high mechanical strength. A stiff structure is ob- served when aromatic or heterocyclic rings are incorporated in the chain skeleton, and when weak C-H bonds are replaced by the stronger C-0 and C-N bonds. This is the background for the synthesis of novel polymeric families that withstand high temperatures (so-called HT polymers).
3.2 THE MOLECULAR ARCHITECTURE
The molecular architecture defines the geometry of the chain. In general, the polymer chain is described by a coil that is capable of adopting various forms in accordance with the ambient conditions, solvents, and temperature. Under conditions where there is no net interaction with the surroundings (so-called theta state, or temperature), a model of a randomly condensed coil
3.2 The Molecular Architecture [ 35 ]
R = end-to-end distance I
Branched Cross linked
Condensed Expanded Coil Coil (theta)
FIGURE 3-1 Polymer chain dimensions
is postulated which is capable of opening and expanding with temperature rise or the use of a better solvent. Hence, the same chain may comprise various volumes under different conditions, where the linear dimension is best represented by the end-to-end distance. This must be taken into account in the case of molecular weight determination when measuring the viscosity of dilute solutions. In rare cases, the chain may be represented by a stiff rod, mostly found in bio-polymers (like DNA and others). See Figure 3-1.
According to the steric structure there can be three major configura- tions-a linear chain, a branched chain, or a cross-linked (network or 3- dimensional) chain, as shown in Figure 3-2. The linear chain has no branches or chemical links with neighboring chains (albeit with the existence of physi- cal links, called entanglements).
The branched chain contains side subchains, mainly obtained by the chain transfer mechanism. Most branches are short but yet are able to de- crease the crystallinity in the polymer, due to steric hindrance. Existence of longer branches affects the flow properties by decreasing viscosity. This
FIGURE 3-2 Steric structure of chains
[ 36 ] Structure and Characterization of Polymers
P FIGURE 3-3 A zigzag structure of PE
improves workability both in melt or solution. However, extremely long branches (of the same order of magnitude as the main backbone) can reverse the effect by increasing viscosity caused by entanglements between adjacent branches. A similar effect is observed when the branches are reactive, such as polyfunctional groups in a condensation reaction which lead to primary intermolecular ties. This represents the third steric structure, the cross- linked chain. Here a lattice network structure is obtained by primary bonds. By increasing the degree of cross-linking, the chain gradually loses its mo- bility and capability to dissolve and it finally reaches the thermosetting state. In this case, the molecular weight and viscosity reach mfinity. In intermedi- ate conditions there appear soluble and nonsoluble phases, which may be separated, named sol and gel, respectively. In true cross-linking, there appears to be no dissolution, but the gel may swell under the effect of solvents. Needless to say, only linear or branched chains show flow properties (thermo- plastics).
The highly ordered planar structures, as obtained by stereospecific po- lymerization, were mentioned in Section 2.3. In contrast to the branched chains, we deal here with linear chains where side substitute groups appear regularly on the same side of the plane, or alternatively. These structures are named isotactic or syndiotactic, respectively, and the degree of order is termed tacticity. In both cases, good conditions for crystallization exist, even when the polymer itself is known as difficult to crystallize (as in the case of polystyrene or polymethylmethacrylate). Any orderless structure is named atactic.
Another look at the geometric structure of polymer chains may show ordered domains like helical coils, wherein the bond and rotation angles are predetermined. Isotactic polypropylene, as an example, possesses a rotation angle 120, so that the structure repeats itself after each three mers. In sim- pler cases, a zigzag structure prevails with a constant bond angle (mostly tetrahedrons with an angle of 109S0), as in polyethylene [See Figure 3-3).
A rotational angle between Oo and the 180 prevails in most cases, thus affecting the practical dimensions of the chains, namely, the end-to-end dis- tance. The most remote distance appears in the trans configuration, and shortest distance is in the cis configuration. The stiffness of the chain and the ambient conditions (temperature) affect the configuration of the chain and, as a result, its properties.
3.3 Molecular Weights and Their Distribution [ 37 1
3.3 MOLECULAR WEIGHTS AND THEIR DISTRIBUTION
High molecular weight represents the most important parameter of mac- romolecules. One can never expect, however, to find chains of uniform size in industrial manufacture. In reality, chains of various lengths are present, so that only an average molecular weight can be determined. Full characteriza- tion would require the width of the molecular weight distribution, as well.
This makes the distinct difference between the meaning of molecular weight in the case of macromolecules and the constant unique values of molecular weight for small molecules. Another complexity comes from the choice of the mode of averaging. As is well known in statistics, there are many ways of averaging, while in a heterogeneous ensemble each average has a different value.
Taking, for example, a simple polymeric chain such as polyethylene, the number n of repeating units (mers), defines the chain length. In polymer science, this is termed Degree of Polymerization (DP).
(CH2-CH2), DP = n
In order to express molecular weight (MW) of the polymer, the DP is multiplied by the molecular weight of the repeating unit. In this case it is (CHz-CH2) = 28. So, if we have DP = 1,000, then MW = 28,000. That would be the case, if we could assume a smgle unique value for DP. As mentioned before, however, that does not happen in most practical cases.
From all the averaging methods, it is customary to use the number- average, M,, and weight average, mW, which are both well defined in a mathe- matical way.
- nlMl + nzM2 + . . . + n N M N - CniMi - CW, M, = - - n l + n 2 + . . . + nN Cni fl
where ni = number of molecules (or moles), of constant MW = Mi. This method actually counts the number of chain groups of definite length.
where Wi = welght of a chain that has MW = Mi. The relationship between weight (Wi) and number (n,) of the chains is simply expressed by
Wi = niMi.
It is easy to prove that, by definition, Mw 1 Mn.
[ 38 ] Structure and Characterization of Polymers - -
Therefore, the ratio MJM, may serve as a measure of the breadth of the distribution. It is customary to prefer the use of mole fractions (x) or weight fractions (w), that sum to unity Ex, = Cwi = 1. A general expression may represent various averages, as follows:
This enables the use of some higher moment averages like and Mz+ ,. x = 1;M = M, (numberaverage) x = 2; Ei = Mw (weight average) x = 3;M = Mz (zaverage) x = 4; M = ?Viz+, (z + 1 average)
While the two higher moment averages (z, z + 1) are more sensitive to the existence of very long tails only the first two averages ordinarily have physi- cal significance. In order to stress the difference between the two major aver- ages, let us look at a numerical (but artificial) example. Suppose that a poly- mer consists of lo3 chains of M1 = lo6, and IO3 chains of M2 = lo4. Then
- io3 - io6 + io3 io4 = 505000
io9 106 + io7 - io4 109 + io7
M, = 2000
(W, = 109;Wz = lo7) Wi = niMi
= 990200 990000 Mw =
In this example, the difference between the two averages stems from the fact that, in the case of Mw, the chains are weighed, while for M, they are only counted. It is obvious that Mw must be sensitive to the very long chains (that weigh more) and Mw is closer to M1 (the higher MW group). The ratio Mw/M, = 1.96, which is close to the statistical value of 2.0. This molecular weight distribution (MWD) is considered to be narrow, whereas in practice a hlgh value (broad distribution) is sometimes met. (For example, up to 40-50 for low density polyethylene, LDPE.)
Taking a binary mixture of the same weight, say lkg of each group, the new M, will be different.
= 19800. whereas Mw = 505000 - CWi - 2 M, = - - wi 1 1 c- - + - M~ 106 1 0 4
It is clearly understood that %in is more sensitive to the existence of the short chains (the less heavy).
3.3 MOkCdar Weights and Their Distribution
We can now plot a "normal" distribution curve, as W(M), which means weight fraction per unit molecular weight, versus M. This provides us with the best information regarding the shape of MWD and the exact location of each average. In this curve, we incorporated another average (actually a range of averages), - named mv (viscosity average molecular weight). See Figure 3-4.
M, is determined by measuring the viscosity of a polymer dilute solution, and using appropriate correlations between the so-called intrinsic viscosity of the polymer in the solution [p] and the molecular weight. This is defined as follows:
[ 39 ]
p = viscosity of solution at concentration C. p, = viscosity of the pure solvent.
M - M, e< mv e mw (Closer to mw )
A = Narrow MWD B = Broad MWD
FIGURE 3-4 A differential MWD curve
[ 40 ] Structure and Characterization of Polymers
The value of intrinsic viscosity is reached upon extrapolation to infinite dilution (C = 0).
The empirical relation between [p] and M is named after Mark and Hou- wink (the M-H equation):
[p] = K Wv (3-5)
Such an expression may be linearized on a log-log scale, where a = the slope of the straight line. The common range for the exponent, a, lies lietween 0.5 and 0.8.
Finally, the viscosity average molecular weight, Mv, is defined:
- When a = 1, Mv = M,, so that Mv is usually close to M,, but its value depends on the parameter a, and hence one observes a range of E., (as shown in the graph, Figure 3.4). However, Mv will approach Bn, only if one predicts a hypothetical value for a = - 1. The parameters K and a, for each pair of polymer-solvent (at a given temperature), are found by calibrating with nar- rowly distributed polymer samples (fractions), for which M (prefer E,) is given. Much data can be found in handbooks.
The intrinsic viscosity (IV) is physically related to the hydrodynamic volume of the chain (its volume during flow), so that when the chain dimen- sions (as defined by end-to-end distance) increase in the solution, the IV will increase en suite. In practice, a large deviation is found between IV in a bad solvent (worst conditions at the so-called theta (0) state, where a = O S ) , and in an excellent one [where high values of IV are found and a = 0.8).
The theta state is defined for the polymer-solvent system (only in case of poor solvents) as that temperature where minimal interaction between the chain and its environment prevails. This is also defined as the threshold limit of dissolution (at high molecular weight) and the chain takes on a configuration of a dense coil.
The correlation between IV and the chain dimension in solution is best expressed by Florys universal expression:
[p] = AR3/M = BVlM (3-7)
In this equation A and B represent universal constants, R represents a typical linear dimension of the chain (usually the end-to-end distance), and V = hydrodynamic volume of the chain in solution. One may assume that the product [p] M is associated with the volume of the chain. This assumption will be undertaken in a later discussion of MWD utilizing a size separation technique (GPC).
The measurement of intrinsic viscosity is performed in a capillary viscom-
3.3 Molecular Weights and Their Distribution
eter (mostly made of glass) which determines the flow times of the pure solvent and those of the polymer solution at various concentrations (in the diluted region). The ratio of flow times, between the polymer solution and the pure solvent, approximates the viscosity ratio (relative viscosity, pr)
The term psp (specific viscosity) expresses the relative contribution of the polymer to the viscosity of the solution.
It is customary to measure the viscosity of a polymer melt (at high temper- ature), p, , which is very sensitive to MW.
-3.4 F O = AM, (3-10)
Here, po represents melt viscosity under low shear conditions (the Newtonian range).
More details about the viscosity are described in Chapter 4, which deals with rheology of polymers. The industry prefers to measure melt fluidity (inverse viscosity), by using a standard rheometer, named Melt Flow Indexer. The measured property (mass of polymer that flows through a standard capil- lary under determined load and temperature, for 10 minutes) is also known as MFI (Melt Flow Index). Because MFI is inversely related to melt viscosity, it is important to remember that low values of MFI are obtained by high MW polymers.
There are various experimental methods for the assessment of MW aver- ages. We will describe some that are absolute and need no calibration. The number average, Mn, can be obtained, in principle, by utilizing common methods of general and organic chemistry-elevation of boiling point, sup- pression of melting point, and reduction of vapor pressure (the so-called col- ligative properties). The major deficiency stems from the fact that when increasing the molecular weight it becomes more difficult to measure the diminishing changes in temperature or pressure. If, for example, a low con- centration of 0.01 molar is used, one needs a solution of 100 glL for M = lo4 and 1,000 glL for M = 10. At these concentrations it is impossible to obtain a polymer solution instead of a gel. On the other hand, further reduction of the molar concentrat ion reduces the measured reading.
Sometimes, it is possible to use the simple method of neutralization of a reactive chemical end group (like COOH in polyester or polyamide). Upon increasing molecular weight, however, the concentration of the reactive end groups diminishes significantly. Therefore, the use of these methods is lim- ited to the range of mn < 20,000. Above that value, it is customary to mea-
[ 42 ] Structure and Characterization of Polymers
FIGURE 3-5 Osmotic pressure of polymer solutions
sure the osmotic pressure formed when a dilute polymer solution is separated from the pure solvent by a semipermeable membrane. The simple relation- ship between the osmotic pressure (.) and the other variables (molecular weight M, concentration C, and temperature T) is described by the next expression. See Figure 3-5.
_ - n - RT - (A + BC) C
The coefficient B (so-called second virial) depends on the thermodynamic interaction between the polymer and the solvent. It vanishes at the theta condition, which leads to the Van't Hoff equation, commonly used in general- chemistry . = (CRT)/M.
The same expression is obtained after extrapolation to C = 0, the limiting absolute value for M,. The number average molecular weight, as measured by this method, is frequently utilized in polymer science, in the region of M, = 2 lo4 - 5 * lo5. Below this region, a false reading may result, due to the possible passage of short chains through the membrane. In order to avoid this discrepancy, good selectivity of the membrane is essential.
The weight average is obtained by measuring the light scattering in poly- mer dilute solution at various concentrations in a photoelectric cell. High clarity and purity of the solution is crucial for obtaining accurate results. The observed parameter is the "turbidity" coefficient, T, which is related to MW according to the following expression:
- = - HC I + 2BC T M (3-12)
Constant B is identical to that in Equation (3-1 1). H represents a combination of optical parameters, fixed for the system. Again, the constant B vanishes at
3.3 Molecular Weights and Their Distribution
theta condition, eliminating the need of measuring at several concentrations. As mentioned, this method is very sensitive to contaminants and dust, and it is often necessary to measure at several angles and at various concentrations.
Except for research laboratories, it is uncommon in industry to utilize the exact absolute methods for molecular weight estimation. Instead, it is common to measure the viscosity of a single concentration solution, or the melt, usually the MFI. In quality control, one is concerned with fluctuations rather than absolute values.
Since the mid 1960s, a new instrument has been developed called GPC (Gel Permeation Chromatography), which provides the molecular weight dis- tribution curve as well as all the averages. This method is based on liquid chromatography, giving exact information about the concentration of chains of varying length, according to the elution time, after flowing in dilute solu- tion through packed columns filled with well-defined porous gels. See Figure
It is interesting to note, that the shortest chains (including the solvent itself) undergo the longest route through the internal pores while the longest chains (unable to penetrate into the gel pores) are rejected and emitted earlier. By appropriate calibration, the chromatogram is converted to a true (finger- print) molecular weight distribution curve, from which all pertinent averages are easily calculated. The most reliable calibration is based on the relation- ship between the product [p]M (intrinsic viscosity multiplied by molecular weight) and elution volume (or time), following Florys equation (3-7) which relates intrinsic viscosity to hydrodynamic volume and molecular weight. This may be described by the universal calibration curve, a straight line on a semilogarithmic scale. See Figure 3-7.
In research and development the characterization of polymers, as regards to molecular weight averages and distribution, is essential in order to predict
[ 43 ]
small molecules (solvent)
FIGURE 3-6 Separation in CPC columns
[ 44 ] Structure and Characterization of Polymers
elution volume V (time)
FIGURE 3-7 Universal calibration curve for GPC rneasu remen ts
the relationship between the molecular structure and polymer performance. In industry it is important to follow polymer characterization in view of controlling the homogeneity in production and deriving improved perfor- mances. In general, many properties are improved by an increase in molecular weight but it becomes difficult to process polymers exhibiting very long chains. A typical example is the UHMW (ultra high molecular weight) poly- ethylene used for very thin plastic bags. Enhanced mechanical properties can he obtained, but at the price of convenience in fabrication. As for the width of distribution, it is well known that widely distributed polymers gain better processability, albeit with some drop of mechanical properties.
Most physical properties (including viscosity) are related to the weight average, but some are correlated to the number or intermediate averages. It is advantageous to obtain the complete molecular weight distribution data from which the various averages and general equations may be derived (all facili- tated by a good computer).
The performance of polymers may be best understood by considering the concept of thermal transition that determines the transition between phases and states. The primary transition, between a crystalline solid phase and an amorphous liquid (polymers never appear as gases), is defined by the melting point, T,. In this case, genuine changes in the primary thermodynamic prop- erties (enthalpy, specific volume] occur, as with small molecules. The major difference is that in. polymers there is no sharp transition point but a range of temperatures - depending on molecular weight distribution and on the degree of crystallinity (discussed in Section 3.5). In essence, T, defines the disappear- ance of the crystalline phase, being the temperature at which the last crystal- lites melt. It increases with an increase of molecular weight, concentration
3.4 Transitions [ 45 I
and dimensions of the crystallites. It is affected by the rigidity of chemical structure of the chain core, presence of strong intermolecular bonds, and bulky side groups. Needless to say, amorphous polymers lack the primary transition and, therefore, have no melting point. They soften upon heating, however, and soliddy glasslike at low temperatures. The amorphous phase, however, exhibits a secondary transition temperature of extreme signifi- cance, the so-called glass transition temperature, T,. It is named secondary (in spite of primary importance), due to the fact that a step-change of secondary thermodynamic properties occurs (such as thermal expansion coefficient or specific heat), representing the temperature derivatives of primary functions. Therefore, T, corresponds to a change in the slope of the thermodynamic function with temperature, as shown by the plot in Figure 3-8.
A glass transition occurs for an amorphous polymer when the slope of a plot of specific volume changes abruptly with rise of temperature. The slope itself (the thermal expansion coefficient a) , a = (1N) dVldT, shows a step- change at T,. A crystalline polymer also shows a transition at the same temperature, due to its amorphous phase. (It will be explained later that only semi-crystallinity may exist and there are almost always amorphous domains.) In the case of a crystalline polymer, however, a primary transition temperature, T,, exists, signified by an abrupt change in volume. The specific volume of the crystalline polymer is always lower than that of the equivalent amorphous one because its more compact structure increases the density.
Many physical properties change in the vicinity of T, (it is really a region), the most prominent being the dynamic ones. A transition between two dy- namic states occurs in the amorphous phase-between the glassy state, wherein the mobility of chain fragments is frozen [frozen free volume) and the elastic state wherein the chain mobility increases upon the rise of temper- ature (the free volume increases and viscosity decreases, respectively). (Free volume is defined as the difference between the volume of the liquid phase and the extrapolated value at absolute zero temperature.) It is customary to define the transition (T,) when a fraction of frozen free volume of 2.5% ap- pears, and stays constant at lower temperatures. There is no real solidifica- tion, however, but a frozen liquid. The rate of the measurement (or the fre-
FIGURE 3-8 Transition temperatures
[ 46 I Structure and Characterization of Polymers
a = T m I
FIGURE 3-9 Multiple transitions
quency) is of importance, showing that the transition is basically dynamic in nature, a state of relaxation. It is therefore advised to gain accuracy by mea- suring at a low rate of temperature changes, as the values of Tg increase with higher rates of measurements. Actually, some more transition temperatures may be found (both below and above Tg) by applying a dynamic test under a wide range of temperatures. If one plots the ' loss factor" (described in Section 4.1) in a dynamic test (mechanical or electrical), several peaks appear, describ- ing very clearly the existence of transitions. The upper one (only in the case of a semicrystalline polymer) represents T,, and then Tg, but also T,,which is related to the release of some degrees of freedom, or mobility, at a lower temperature. See Figure 3-9.
The existence of T, (or other transitions) is associated with the rotation of side groups or other well defined fragments of the mer, thus releasing some additional frozen free volume at temperatures below Tg. It is obvious, that the various transition temperatures have a paramount effect on the polymer performance. Around Tg many parameters are drastically changing, such as
Mod u I us G
FIGURE 3-10 Changes in modulus around T,
3.4 Transitions [ 47 ]
the modulus of rigidity, G, (see Figure 3. lo), coefficient of diffusion, viscosity, and light refraction index. It is believed that the melt viscosity of polymers at T, is about lOI3 poise (very high).
Above T, amorphous liquid appears, while a semi-crystalline solid ap- pears below T,. Above Tg , the amorphous phase shows a high mobility leading to high elasticity and deformity. On the other hand, below Tg most polymers behave like rigid solids, and are frequently brittle (glass-like). Exten- sivity is drastically reduced, together with the capacity to resist the effect of blows and oscillation (impact strength).
Therefore, polymers that have a low T, (compared to service temperature) behave rubber-like or leather-like, with high toughness. Most prominent are the polyolefins and rubber (both synthetic and natural). Other polymers ex- hibit relatively high values for T,, like PS, PVC, PMMA, PC and others. In principle, these polymers are predicted to perform at room temperature as rigid, with low deformability and with a tendency to brittleness. Some are exceptions, however, like PC (polycarbonate) which is very tough in spite of the existence of a rather high Tg (around 15OOC). It has been postulated that the expected brittleness at room temperature is eliminated due to the appear- ance of another transition temperature, T, at ( - 100OC).
For most engineering polymers a high T, (above 100OC) is required, whereas elastomers (synthetic rubbers) need low Tg (usually below - 5OOC). It is also possible to reduce T, by external plasticification (addition of plasti- cizers which generate a solid solution with organic liquids of very low transi- tion temperatures) or by polymerization with other comonomers which leads to lower transitions.
Empirical mixing equations may be useful in this case, like:
(Note: Tg must be expressed at absolute temperature.) W, and W2 represent weight fractions of the appropriate components in the mixture or in the copolymer, respectively. By computing the additivity of free volumes it is possible to gain higher accuracy. It is important to note that T,, in a way similar to T,, is affected by various parameters - molecular weight, degree of crystallinity, rigidity of the chemical structure, and secondary bonds. It is therefore not surprising to find a narrow range for the ratio (in absolute temperatures) TJT, between 1/2 and 2/3 for many polymers. This enables initial estimation of a transition temperature if only one of the two is given. There are many exceptions, however, to this simple empirical rule. It is also possible to predict Tg of a new polymer, from its chemical structure, by adding contributions of various structural units. It is interesting to observe the dependence of T, on the chemical structure, as shown by the following cases:
[ 48 Structure and Characterization of Polymers
Polyethylene, PE -CHZ-CHZ-
T, = -120OC
Polypropylene, PP -CH-CH2-
T, = -17OC
Polyvinylchloride, PVC Polystyrene, PS -CH-CHz- -CH-CHZ-
I I C1
T, = +87OC C6H5
Tg = +lOOC
Therefore, PS is a rigid (high modulus) but a brittle polymer, because of the presence of,a bulky phenyl side group. It can be modified by an elasto- meric phase (usually by copolymerizing), thus augmenting its impact strength. PVC is also rigid with a low impact strength, unless it is modified. It is customary, however, to plasticize PVC by external plasticizers or by copolymerization (with vinyl acetate, for example). The large difference be- tween the values of T, for PE and PVC, is related to the existence of polar forces in PVC.
In conclusion, the existence of various transition temperatures indicates different states in the matter, where T, and T, represent the more important ones having thermodynamic significance. T, is still considered the most dom- inant one, dictating the mechanical and dynamic behavior. Its values appear in various equations as "corresponding states," such as universal parameters at identical TlT, or (T - T,). This idea will be developed further in a discus- sion on viscoelasticity. (See Section 4.1). Table 3-1 exhibits transition temper- atures of some selected polymers.
TABLE 3-1 Transition Temperatures of Some Polymers
Polymer TRoC T,OC
Polyethylene - 120 137 Polypropylene - 17 176 Polybutene- 1 - 25 125
PVC 87 212* Polystyrene 100 240 Polycarbonate 150 250 Nylon 6-6 50 265
'Only for isotactic (crystalline).
Polyisobutylene - 73
3.5 Morphology [ 49 I
Morphology deals with the structure in the solid state. There is a distinct indication that in principle regular polymers are apt to crystallize-meaning to form long-range spatial order. There is an apparent difference, however, between the crystallization of long chains and that occurring in low molecu- lar weight organic or inorganic compounds. In polymers, a complete crystal- line structure is never reached, as noncrystalline (amorphous) regions always interfere. Therefore it is common to use the term semi-crystallinity and to characterize it by degree of crystallinity, defined as the fraction (percentage) of the crystalline phase in the total mass. The theory of polymer structure is a prominent branch of polymer physics, which has mainly developed since the 1950s. It should be mentioned that around 1920 the concept of long chains had been introduced, when X-ray diffraction studies provided the proof for the existence of an ordered crystalline structure. (The intensity of the obtained diffraction rings is measured and the distances apart are transformed into a defined lattice conformation.) It was tacitly assumed that the long chains create a macroscopic structure wherein some regions exhibit order while others do not. (See Figure 3.1 la.) The same long chains pass through the crystalline phases (A) and the amorphous ones (B), alternately. This was described b